Safety assessment of material incompatibility in formulations for pyrotechnic manufacture. Patrick J Sears1, Martyn R Ottaway2, James D Callaway3, James N Towning3 1. 2. 3.
Thermal Hazard Technology, 1 North House, Bond Avenue, Bletchley, UK, MK1 1SW Thermal Hazard Technology inc. 255 Old New Brunswick Road, Suite 120S, Piscataway, NJ. DSTL, Fort Halstead, Sevenoaks, Kent, UK, TN14 7BP
Background ď Ż
The introduction of new pyrotechnic systems requires a structured and progressive safety assessment throughout the initial research then development process.
For new composition formulations an initial rapid and cost effective chemical compatibility screening process is required to act as a 'first sift' to accept formulations for further development.
Full energetic material qualification testing is generally applied much later in the development cycle when a formulation is close to being introduced into an 'in-service' status.
The first experiment with a new pyrotechnic formulation could be a simple ignition pile test to establish if a new pyrotechnic powder actually burns.
However, in order to mix a new pyrotechnic formulation that may contain a new or different ingredients it is necessary to investigate if any chemical compatibility problems exist between fuels, oxidisers and binder systems.
Since a large number of formulation variants and perturbations could be under investigation a rapid screen was thought to be a suitable substitute to full STANNAG compliant testing.
Background ď Ż
If no adverse reaction is evident when comparing individual chemicals with binary and tertiary mixtures small scale mixing can progress for initial trials such as a pile test or small scale burn rate test which can act as a 'second sift'.
A successful candidate formulation may be required to undergo a pressing compaction test followed by a burn rate test ('fourth sift') or larger scale mixing process once a 'third sift' sensitiveness testing has been completed.
Rapid Screening Device (RSD) ď Ż
The RSD is a new calorimeter from Thermal Hazard Technology. Designed as a Process Safety Instrument, this system is a ramped heating technique which allows the users to measure temperature and pressure from samples.
Rapid Screening Device ď Ż
Designed to be fast, accurate yet inexpensive the RSD can use a range of different sample containers to suit a range of applications The RSD is unique as it can handle several samples at the same time giving differential temperature and pressure measurement
How it works….
The RSD is a Ramped Passive-mode Calorimeter (RPmC), which depends on the principles of heat flow and transient heat accumulation. The key to this technique is a very stable heat transfer coefficient. The heat transfer capacity can thus be modelled successfully during the entire reaction period. The RSD measures temperatures and pressures, and as such is capable of providing a real-time basis for determining the partial pressures resulting from condensable vapours and non-condensable gases.
Ramped Passive-mode Calorimetry
RPmC’s successful implementation requires an environment whereby small control changes are applied over relatively long (with respect to a system’s time constant) periods. This ensures smooth transitions to the heat transfer capabilities of each particular test-cell and allows predictions to be made regarding the nature of heat accumulation and heat flow to and from the sample under investigation.
Ramped Passive-mode Calorimetry ď Ż
Understanding the test-cell thermal transfer behaviour provides the basis for the determination of process heats (melting, boiling, reaction, etc.) as well as the determination of thermal transfer based kinetics.
It is also imperative that the heat flow to the sample during the inert pre-process and post-process phases is also quantified successfully. RPmC may also be used to determine heat capacities of unknown samples when referenced against known standards.
For a successful data analysis, certain physical data must be known. The mass and heat capacity of the sample, as well as the test-cell must be known. An air reference temperature is also a prerequisite. This provides a means of calibrating the test-cell during a temperature ramp.
Experimental Phases During an exothermic process, three distinct regimes exist :1. Heat supplementation phase. Here heat is constantly added to the sample from the external temperature. Heat accumulation is due in part to the reaction in progress as well as the power being supplied to maintain the ramp. The power supplied is gradually lessening due to a decreasing temperature difference between the sample and environment. 2. Heat overload phase. At this stage the heat being produced exceeds the capacity of the test-cell to loose it to the environment resulting in an accumulation of heat within the sample. The amount of heat lost to the environment controlled by the heat transfer characteristics of the test-cell: environment interface. 3. Heat dissipation phase. With the reaction complete, all that remains is the measurement of the accumulated heat to the environment. This provides the basis of determining when exactly the reaction ceased during the heat overload phase. When the temperature of the calorimeter and test-cell cross over, the sample is being heated externally once again.
Calculation of Heat Transfer ď Ż
During the pre-process and/or post-process stages the heat transfer capability of test-cell i may be defined by equation 1. UA may be assumed static or dynamic (the latter case may be modelled to vary from the pre-process to the post-process value on the basis of conversion). Typically values vary by 2% to 3% and is considered to be mainly due to the effect of changes to the sample.
dT mCpi dt i Tair
Calculation of Thermodynamics
With UA established, it is then possible to determine a total power balance over the entire experiment see equation 2 (n.b. values are with respect to a reference)
This use of a reference also provides the basis for establishing the point at which exothermic (if present) behaviour ceases. It is therefore possible to determine the total heat consumed or generated by a process from equation 3
d( T) UAi dt pi
qramp Equation 2
q pi dt Equation 3
Kinetics ď Ż
Having determined the specific heat of a process, it is possible to use the temperature rates with knowledge of excess power added or deficit power lost to determine the process kinetics. Essentially equation 4 may be used, such that a linearly corrected Wilson plot for reaction order may be used to establish kinetic parameters
dC H Pi dt i
Delta-Temperature & Pressure
Many binder systems used in pyrotechnic compositions negate combustion efficiency and can lead to difficulties to incorporate sufficient oxidant into a formulation to achieve stoichiometric combustion, without compromising physical properties. There is potential to mitigate this problem through the use of energetic polymers such as Poly NIMMO (C5H9O4N, Poly(3methyl-3-nitratomethyl oxetane)) .
The term ‘energetic polymer’ is normally used to describe macromolecules which contain energetic functionalities such as nitrato, nitro or azido groups.
Testing Introduction ď Ż
A series of chemical compatibility tests using the THT RSD have been carried out to investigate using Poly NIMMO energetic binder in pyrotechnic formulations. Poly NIMMO is attractive as en energetic binder which has a standard enthalpy of formation ( H f ) of -337 kJ.mol-1, an oxygen balance of -114.3 and a decomposition energy (DSC) 1300 j/g.
Magnesium powder was used as an example of a metallic fuel and potassium benzoate as an organic fuel.
Potassium and sodium nitrate were selected as candidate oxidiser systems.
Red phosphorus, that is often used in military pyrotechnic smoke compositions was also selected since its chemical reactivity is prone to degradation reactions during storage, which potentially can make it more difficult to ignite, reduce its burn rate and lead to the evolution of toxic phosphine.
Phosphorus in Compositions ď Ż
Red phosphorus systems typically utilise minimal quantities of inert binders; however, this can make it difficult to coat the individual particles sufficiently to quench their chemical reactivity. The use of energetic binders such as Poly NIMMO in pyrotechnic compositions should permit the use of higher percentages of binder than those normally employed with inert binders, so generating a thicker protective polymer layer around individual phosphorus particles.
As the energetic binder will itself burn (even in absence of air) phosphorus combustion should be promoted, thereby enhancing burn rate/thermal output of the device.
The samples were prepared using the incipient wetness technique. The support material was dried for at 110°C to remove all water. The sample was then wetted with acetone to determine the volume of water adsorbed per gram of support. Once this had been determined, a solution of the energetic binder in acetone of the appropriate molarity was produced. A second dried sample of support material was then wetted using this solution and then dried for 24 hours at 70°C.
Initial screening experiments were first conducted in Glass Vials however these were abandoned as ignition events could give rise to cell rupture. The samples were mounted in small glass ignition tubes within the test cell to avoid the influence of metal on the tests.
Identical conditions have been utilised for all the tests conducted here with a sample mass of 0.15g. The tests were conducted from room temperature to 400°C at a scan rate of 4°C/min.
In the worst cases the tests were terminated abnormally because of the high energies involved.
Example results from Standard Materials with PolyGlyn
Example results from Standard Materials with PolyGlyn
Results – Standard Materials
All the results observed show a low heat transition at ca. 180°C. This is accompanied by a small increase in the pressure. All other endotherms and exotherms observed are unique to the materials being tested but are consistent with literature transitions for the materials
Exploring the effect of the binder - Poly NIMMO & NaNO3
Without Poly NIMMO
Without Poly NIMMO
With Poly NIMMO
With Poly NIMMO
Results – The binder effect
The results from the previous slide, comparing the analysis of NaNO3 with and without PolyNIMMO show no incompatibilities between the materials.
The result from the PolyNIMMO coated material shows the same features as the uncoated material with the additional temperature generation from the binder and an associated rise in the observed pressure.
Full Compatibility test ď Ż
To fully explore the compatibility of a single test system one, three component formulation (with energetic binder) was chosen for study. Full results are shown below for binary and tertiary mixtures of NaNO3, Red Phosphorus and Magnesium powder together with Poly NIMMO as an energetic binder.
Mg and NaNO3
Red Phosphorus & Mg
Red Phosphorus & NaNO3
All Three Componentsâ€Ś.
Two ignition type incompatibilities have been observed in these experiments with poly NIMMO bound materials: Rp/NaNO3 (123°C) Rp/NaNO3/Mg (297°C) The RSD has shown how both compatible and incompatible mixtures can be rapidly identified to ensure safe practice in a laboratory environment prior to scaling to fully STANAG compliant testing.
Further simple information: Air temperature record Sample holder mass Sample heat capacity Would allow information on the nature of the measured events to be quantified (Heat of reaction, Ea, onset kinetics etc)